#------------------------------------------------------------------------------
#$Date: 2024-05-06 07:23:50 +0300 (Mon, 06 May 2024) $
#$Revision: 291734 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/30/07/2300736.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2300736
loop_
_publ_author_name
'Shtender, Vitalii'
'Cedervall, Johan'
'Ek, Gustav'
'Zlotea, Claudia'
'Andersson, Mikael S.'
'Manuel, Pascal'
'Sahlberg, Martin'
'Häussermann, Ulrich'
_publ_section_title
;
 Revisiting the hydrogenation behavior of NdGa and its hydride phases.
;
_journal_coeditor_code           NB5371
_journal_issue                   'Pt 2'
_journal_name_full               'Journal of applied crystallography'
_journal_page_first              248
_journal_page_last               257
_journal_paper_doi               10.1107/S1600576724000554
_journal_volume                  57
_journal_year                    2024
_chemical_formula_sum            'Ga Nd'
_chemical_formula_weight         213.96
_space_group_crystal_system      orthorhombic
_space_group_IT_number           63
_space_group_name_Hall           '-C 2c 2'
_space_group_name_H-M_alt        'C m c m'
_atom_sites_solution_primary     20
_audit_creation_method           SHELXL-2019/1
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.4329(12)
_cell_length_b                   11.246(3)
_cell_length_c                   4.1735(11)
_cell_measurement_reflns_used    2217
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      31.719
_cell_measurement_theta_min      3.623
_cell_volume                     208.06(10)
_computing_structure_refinement  'SHELXL-2019/1 (Sheldrick, 2019)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker D8'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0296
_diffrn_reflns_av_unetI/netI     0.0180
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_number            2217
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         31.719
_diffrn_reflns_theta_min         3.623
_exptl_absorpt_coefficient_mu    37.104
_exptl_absorpt_correction_T_max  0.698
_exptl_absorpt_correction_T_min  0.641
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_density_diffrn    6.830
_exptl_crystal_description       needle
_exptl_crystal_F_000             364
_exptl_crystal_size_max          0.03
_exptl_crystal_size_mid          0.01
_exptl_crystal_size_min          0.01
_refine_diff_density_max         0.933
_refine_diff_density_min         -1.246
_refine_diff_density_rms         0.238
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_goodness_of_fit_ref   1.107
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     10
_refine_ls_number_reflns         220
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.107
_refine_ls_R_factor_all          0.0225
_refine_ls_R_factor_gt           0.0147
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0044P)²+0.5138P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0193
_refine_ls_wR_factor_ref         0.0201
_reflns_Friedel_coverage         0.000
_reflns_number_gt                187
_reflns_number_total             220
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            nb5371sup1.cif
_cod_data_source_block           NdGa
_cod_depositor_comments
;Adding full bibliography for 2300736--2300740.cif.

 Adding full bibliography for 2300736--2300740.cif.
;
_cod_database_code               2300736
_cod_database_fobs_code          2300736
_shelx_shelxl_version_number     2019/1
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x, y, -z+1/2'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z-1/2'
'x, -y, z-1/2'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z-1/2'
'x+1/2, -y+1/2, z-1/2'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Nd1 Nd 0.000000 0.35806(3) 0.250000 0.01023(11) Uani 1 4 d S T P . .
Ga2 Ga 0.000000 0.07009(6) 0.250000 0.01126(14) Uani 1 4 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nd Nd -0.1943 3.0179 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Ga2 Nd1 Ga2 150.26(3) 13_556 13_455 ?
Ga2 Nd1 Ga2 89.45(2) 13_556 13_456 ?
Ga2 Nd1 Ga2 82.99(2) 13_455 13_456 ?
Ga2 Nd1 Ga2 82.99(2) 13_556 13 ?
Ga2 Nd1 Ga2 89.45(2) 13_455 13 ?
Ga2 Nd1 Ga2 150.26(3) 13_456 13 ?
Ga2 Nd1 Ga2 104.868(14) 13_556 . ?
Ga2 Nd1 Ga2 104.868(13) 13_455 . ?
Ga2 Nd1 Ga2 104.868(13) 13_456 . ?
Ga2 Nd1 Ga2 104.868(14) 13 . ?
Ga2 Nd1 Ga2 48.161(15) 13_556 5 ?
Ga2 Nd1 Ga2 106.928(18) 13_455 5 ?
Ga2 Nd1 Ga2 106.928(17) 13_456 5 ?
Ga2 Nd1 Ga2 48.161(15) 13 5 ?
Ga2 Nd1 Ga2 137.092(14) . 5 ?
Ga2 Nd1 Ga2 106.928(17) 13_556 5_455 ?
Ga2 Nd1 Ga2 48.161(15) 13_455 5_455 ?
Ga2 Nd1 Ga2 48.161(15) 13_456 5_455 ?
Ga2 Nd1 Ga2 106.928(17) 13 5_455 ?
Ga2 Nd1 Ga2 137.092(14) . 5_455 ?
Ga2 Nd1 Ga2 85.82(3) 5 5_455 ?
Ga2 Nd1 Nd1 54.742(13) 13_556 9_566 ?
Ga2 Nd1 Nd1 98.493(19) 13_455 9_566 ?
Ga2 Nd1 Nd1 54.742(13) 13_456 9_566 ?
Ga2 Nd1 Nd1 98.493(19) 13 9_566 ?
Ga2 Nd1 Nd1 146.831(12) . 9_566 ?
Ga2 Nd1 Nd1 52.185(14) 5 9_566 ?
Ga2 Nd1 Nd1 52.185(14) 5_455 9_566 ?
Ga2 Nd1 Nd1 98.493(19) 13_556 9_565 ?
Ga2 Nd1 Nd1 54.742(13) 13_455 9_565 ?
Ga2 Nd1 Nd1 98.493(19) 13_456 9_565 ?
Ga2 Nd1 Nd1 54.742(13) 13 9_565 ?
Ga2 Nd1 Nd1 146.831(12) . 9_565 ?
Ga2 Nd1 Nd1 52.185(14) 5 9_565 ?
Ga2 Nd1 Nd1 52.185(14) 5_455 9_565 ?
Nd1 Nd1 Nd1 66.34(2) 9_566 9_565 ?
Ga2 Nd1 Nd1 156.265(18) 13_556 13_455 ?
Ga2 Nd1 Nd1 53.471(18) 13_455 13_455 ?
Ga2 Nd1 Nd1 96.581(19) 13_456 13_455 ?
Ga2 Nd1 Nd1 101.864(18) 13 13_455 ?
Ga2 Nd1 Nd1 51.397(13) . 13_455 ?
Ga2 Nd1 Nd1 147.605(9) 5 13_455 ?
Ga2 Nd1 Nd1 93.99(2) 5_455 13_455 ?
Nd1 Nd1 Nd1 144.622(11) 9_566 13_455 ?
Nd1 Nd1 Nd1 103.249(18) 9_565 13_455 ?
Ga2 Nd1 Nd1 96.581(19) 13_556 13 ?
Ga2 Nd1 Nd1 101.864(18) 13_455 13 ?
Ga2 Nd1 Nd1 156.265(19) 13_456 13 ?
Ga2 Nd1 Nd1 53.471(18) 13 13 ?
Ga2 Nd1 Nd1 51.397(13) . 13 ?
Ga2 Nd1 Nd1 93.99(2) 5 13 ?
Ga2 Nd1 Nd1 147.605(9) 5_455 13 ?
Nd1 Nd1 Nd1 144.622(11) 9_566 13 ?
Nd1 Nd1 Nd1 103.249(18) 9_565 13 ?
Nd1 Nd1 Nd1 69.36(2) 13_455 13 ?
Ga2 Nd1 Nd1 101.864(18) 13_556 13_456 ?
Ga2 Nd1 Nd1 96.581(19) 13_455 13_456 ?
Ga2 Nd1 Nd1 53.471(18) 13_456 13_456 ?
Ga2 Nd1 Nd1 156.265(18) 13 13_456 ?
Ga2 Nd1 Nd1 51.397(13) . 13_456 ?
Ga2 Nd1 Nd1 147.605(9) 5 13_456 ?
Ga2 Nd1 Nd1 93.99(2) 5_455 13_456 ?
Nd1 Nd1 Nd1 103.249(18) 9_566 13_456 ?
Nd1 Nd1 Nd1 144.622(11) 9_565 13_456 ?
Nd1 Nd1 Nd1 64.782(19) 13_455 13_456 ?
Nd1 Nd1 Nd1 102.79(3) 13 13_456 ?
Ga2 Ga2 Ga2 105.86(5) 9 9_556 ?
Ga2 Ga2 Nd1 133.103(17) 9 13_556 ?
Ga2 Ga2 Nd1 68.038(16) 9_556 13_556 ?
Ga2 Ga2 Nd1 68.038(16) 9 13_455 ?
Ga2 Ga2 Nd1 133.103(16) 9_556 13_455 ?
Nd1 Ga2 Nd1 150.27(3) 13_556 13_455 ?
Ga2 Ga2 Nd1 133.103(16) 9 13_456 ?
Ga2 Ga2 Nd1 68.038(16) 9_556 13_456 ?
Nd1 Ga2 Nd1 89.45(2) 13_556 13_456 ?
Nd1 Ga2 Nd1 82.99(2) 13_455 13_456 ?
Ga2 Ga2 Nd1 68.038(16) 9 13 ?
Ga2 Ga2 Nd1 133.103(17) 9_556 13 ?
Nd1 Ga2 Nd1 82.99(2) 13_556 13 ?
Nd1 Ga2 Nd1 89.45(2) 13_455 13 ?
Nd1 Ga2 Nd1 150.27(3) 13_456 13 ?
Ga2 Ga2 Nd1 127.07(2) 9 . ?
Ga2 Ga2 Nd1 127.07(2) 9_556 . ?
Nd1 Ga2 Nd1 75.133(14) 13_556 . ?
Nd1 Ga2 Nd1 75.133(13) 13_455 . ?
Nd1 Ga2 Nd1 75.133(13) 13_456 . ?
Nd1 Ga2 Nd1 75.133(13) 13 . ?
Ga2 Ga2 Nd1 63.80(2) 9 5_445 ?
Ga2 Ga2 Nd1 63.80(2) 9_556 5_445 ?
Nd1 Ga2 Nd1 131.839(15) 13_556 5_445 ?
Nd1 Ga2 Nd1 73.072(18) 13_455 5_445 ?
Nd1 Ga2 Nd1 73.072(17) 13_456 5_445 ?
Nd1 Ga2 Nd1 131.839(15) 13 5_445 ?
Nd1 Ga2 Nd1 137.093(14) . 5_445 ?
Ga2 Ga2 Nd1 63.80(2) 9 5_545 ?
Ga2 Ga2 Nd1 63.80(2) 9_556 5_545 ?
Nd1 Ga2 Nd1 73.072(17) 13_556 5_545 ?
Nd1 Ga2 Nd1 131.839(15) 13_455 5_545 ?
Nd1 Ga2 Nd1 131.839(15) 13_456 5_545 ?
Nd1 Ga2 Nd1 73.072(18) 13 5_545 ?
Nd1 Ga2 Nd1 137.093(14) . 5_545 ?
Nd1 Ga2 Nd1 85.81(3) 5_445 5_545 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Nd1 Ga2 3.1497(6) 13_556 ?
Nd1 Ga2 3.1497(6) 13_455 ?
Nd1 Ga2 3.1497(6) 13_456 ?
Nd1 Ga2 3.1497(6) 13 ?
Nd1 Ga2 3.2386(12) . ?
Nd1 Ga2 3.2556(8) 5 ?
Nd1 Ga2 3.2556(8) 5_455 ?
Nd1 Nd1 3.8142(10) 9_566 ?
Nd1 Nd1 3.8142(10) 9_565 ?
Nd1 Nd1 3.8954(8) 13_455 ?
Nd1 Nd1 3.8954(8) 13 ?
Nd1 Nd1 3.8954(8) 13_456 ?
Ga2 Ga2 2.6153(9) 9 ?
Ga2 Ga2 2.6153(9) 9_556 ?
